The Young s Modulus of SingleWalled Carbon Nanotubes


 Kelley Hamilton
 1 years ago
 Views:
Transcription
1 The Young s Modulus of SingleWalled Carbon Nanotubes Douglas Vodnik Faculty Advisor: Dr. Kevin Crosby Department of Physics, Carthage College, Kenosha, WI Abstract A new numerical method for calculating the Young s modulus of carbon nanotubes which avoids ambiguities that have plagued other attempts is validated. Molecular dynamics simulations that utilize the Tersoff Potential are used to model various singlewalled carbon nanotubes under different strains to achieve this validation. Data is taken from an armchair, zigzag, and chiral carbon nanotube. The calculated Young s moduli are all around Y = 1 TPa, in agreement with existing experimental data. 1 Introduction Carbon nanotubes (CNTs) were discovered in 1952 by L. V. Radushkevich and V. M. Lukyanovich, but they were not brought to the attention of the scientific community until 1991, when Sumio Iijima discovered CNTs in the soot of graphite electrodes after an arc discharge [1]. Since then, the exciting properties of CNTs have led to a host of proposed applications, many of which are currently being realized. A convenient way to think about CNTs is to think of them as a sheet of graphene rolled up into a tube and capped on either end with a part of a buckyball. Graphene is a hexagonal lattice of carbon atoms connected by sp 2 bonds. Multiple stacked sheets of graphene compose the common form of carbon called graphite. A buckyball is a carbon molecule in the shape of a sphere. The CNT is capped in such a way so that every carbon atom is bonded to three other carbon atoms. The way that the graphene is rolled up determines what is called the chirality of the nanotube. CNTs can be grouped into three categories based on chirality: armchair, zigzag, and chiral (Fig. 1). Armchair CNTs contain carboncarbon bonds which are perpendicular to the tube s axis, while zigzag CNTs contain bonds that are parallel to the tube s axis. Chiral CNTs 1
2 Figure 1: An example of each of the three types of CNT chiralities [2]. contain bonds neither perpendicular nor parallel to the axis of the tube. Each category is named for the nanotubes edge pattern. Each CNT can be uniquely identified with the index pair (n, m), n m. All armchair CNTs have index pairs of the form (n, 0), and all zigzag CNTs have index pairs of the form (n, n). Agreatdealofusefulinformationiscontainedintheindexpair.Forexample,theradiusof a given CNT is r = l 3(n 2 + m 2 + nm) 2π where the carboncarbon bond length l =1.42 Å[3]. Carbon nanotubes demonstrate a number of unique properties. They are the stiffest material known, yet they are also very bendable [4, 5]. CNTs are only a few nanometers in diameter, but they can range in length from a few nanometers to 18 centimeters [6]. Depending on the tube geometry and the strain that the nanotube is experiencing, CNTs can be either metallic or semiconducting [7]. CNTs can also be nested inside one other to create multiwalled carbon nanotubes (MWCNTs). Carbon nanotubes without other nanotubes nested within them are referred to as singlewalled carbon nanotubes (SWCNTs) to differentiate them from MWCNTs. The proposed applications of CNTs promise to affect fields such as nanotechnology, materials science, and electronics [8, 9, 10, 11]. They range from space elevator cables to synthetic muscles [8, 9]. Although many of these applications have not yet come to fruition, advances 2
3 in the application of CNTs have already been made. For example, carbon nanotubes are already used to make various composite materials stronger and more stiff, and their addition to motors and transistors is rapidly allowing motors and transistors to become smaller than they have ever been before [10, 11]. Unfortunately, production and characterization problems currently hinder the advancement of CNT applications. The current method of CNT production, for example, is still relatively primitive. CNTs can easily be produced, but at the moment it is all but impossible to specifically create large quantities of nanotubes with a predetermined chirality or length [12]. Widespread use of carbon nanotubes requires costeffective and reliable methods of production, but at the moment such methods of production have not been discovered. A second problem hindering the application of CNTs is the uncertainty surrounding their mechanical properties. Many of the values that are used to describe mechanical properties of materials have traditionally assumed that the material being described is macroscopic. The microscopic nature of CNTs poses new challenges to the definition of the aforementioned values that have not yet been resolved. In this paper, validation is provided to a new characterization of one of the most important values, Young s modulus, which circumvents many of the problems that have hampered previous attempts to precisely define it. 2 Young s Modulus 2.1 Background Young s modulus is a value associated with a material that represents that material s stiffness. In other words, Young s modulus relates the stress applied to the material with the resulting strain of the material. The Young s modulus of a material must be known before the material can be used in many practical applications, but there is currently disagreement over how to define Young s modulus for carbon nanotubes. This disagreement stems mostly from the fact that Young s modulus is only properly defined for continuous materials, while CNTs are crystalline materials. For continuous, bulk materials, Young s modulus is defined as Y = σ,whereσ is the axial stress and ε is the ε axial strain. Axial stress, in turn, can be written as σ = F,whereF is the force applied A over the crosssectional area A (Fig. 2). Young s modulus, therefore, requires an unambiguous crosssectional area. For continuous materials, defining the crosssectional area is quite simple. For discrete materials such as carbon nanotubes, however, this task is ambiguous. 3
4 Figure 2: Young s Modulus for continuous materials [13]. Axial strain ε = L L,orε = L L Methods of Defining Young s Modulus The crosssectional area of carbon nanotubes is ambiguous for two main reasons. The first reason is that the force is not applied uniformly, but is applied at discrete points due to the CNTs crystalline structure. The second reason is that the discrete points to which the force is applied are distributed around the circumference of the nanotube, not uniformly across the entire crosssectional area. The crosssectional area of CNTs has been defined differently by different researchers. A common definition of the crosssectional area is that of a solid cylinder or prism [14]. Another popular definition of A is that of a hollow cylinder with a thickness [14]. 1 Still others have opted to define the much more straightforward circumference instead of the troublesome crosssectional area [14]. This method views the CNT as basically onedimensional and produces a value called the surface Young s modulus. This surface Young s modulus is applicable in some situations, but it is not the same value as Young s modulus and so doesn t completely solve the original problem of defining Y. 2.3 The Second Derivative of the Strain Energy Density These different methods of defininga predictably produce different values of Young s moduli. Young s modulus is supposed to be a constant of the material, so these attempts to define the crosssectional area seemingly fail. But recently, an application from elastics has led to a new method of defining Young s modulus for CNTs to be proposed. This new method defines Young s modulus as the second derivative of the strain energy density with respect Å is the most common thickness, since it is the distance of separation between layers of graphene in graphite. Other values have also been used, though. 4
5 to the axial strain [14]. This method circumvents the problem of having to define the crosssectional area of CNTs and so has the potential to finally and definitively define Young s modulus. In the case of carbon nanotubes under axial strain, the strain energy of the CNT is its internal elastic potential energy. The internal elastic potential energy U e of a CNT experiencing axial strain is U e = YA L L 0 dl = YA L 0 L dl = YA L2 2L 0 where A is the crosssectional area, L 0 is the initial length, L is the change in length, and Y is Young s modulus. The internal elastic potential energy per unit volume, or the internal elastic potential energy density, can be written as where V = Ue AL 0.Sinceε = L L 0,wecanwrite V = Y L2 2L 2 0 V = 1 2 Yε2 and then take the second derivative or the internal elastic potential energy density, or strain energy density, with respect to strain to find Young s modulus: d2 V dε 2 = Y. 3 Method 3.1 Molecular Dynamics Simulation Molecular dynamics simulations are a type of simulation program that models materials on the molecular scale. These programs first read a potential that describes the interactions between atoms, as well as information on atomics masses, initial positions, and initial velocities. From this information, the programs calculate the force on each atom due to atoms around it. Then, the programs solve for the acceleration of each particle and perform a double integration to find the change in position of each atom. Finally, the programs apply the position changes and repeat the process as many times as required. A molecular dynamics simulation tool called XMD was utilized to create a program that simulates SWCNTs experiencing strain [15]. After creating the nanotube, the program sets the temperature of the nanotube, and also implements the Tersoff Potential to model the 5
6 interactions between the carbon atoms. The program allows the CNT to reach mechanical equilibrium, and then begins to gradually increase the strain that the CNT is under until the CNT reaches maximum strain. 2 Inputs for the final program include chirality, length of CNT, duration of incremental strain increase, maximum strain, and temperature. Outputs include particle displacement, the product of internal stress and atomic volume, and internal potential energy, which in this case is also the strain energy. Data was gathered from three SWCNTs: a (5,5) armchair CNT, a (9,0) zigzag CNT, and a (6,4) chiral CNT. The temperature was set to T =0K. 3.2 Finite Size Scaling Analysis Molecular dynamics simulations produce reliable results only when edges and boundaries are not a significant portion of the material being simulated. In other words, simulations which model materials that are too small usually produce nonphysical results. So, in order to run an efficient simulation that still produces reliable results, the molecular dynamics program should be made to simulate CNTs with the shortest length that still produces realistic data. In order to find this optimum length, finite size scaling analysis is necessary. The XMD program requires that the length of a CNT be inputted in terms of unit lengths that are determined by the program. The length of a unit length changes for each CNT, as it is dependent on chirality of the nanotube. For the (5,5) armchair CNT the unit length is about nm, for the (9,0) zigzag CNT the unit length is about nm, and for the (6,4) chiral CNT the unit length is about nm. Young s moduli for CNTs of unit lengths 17 were calculated (Fig. 3). The Young s moduli for lengths of 13 units were all quite large. Starting with lengths of 4 units, though, the calculated Young s moduli ceased to change dramatically, although they slowly begin to increase. Since CNTs with lengths of 4 units are the shortest CNTs that follow this trend, they are most likely the nanotubes with the smallest length that can reliably model actual CNTs. 4 Results and Analysis After plotting the strain against the strain energy, the second derivative of the graph s best fit parabola was taken to find the product of Young s modulus and atomic volume. 3 The average atomic volume can be easily calculated from the particle displacement data, so it was divided out to calculate Young s modulus. 2 Mechanical equilibrium is defined in this case as the state of the CNT in which the internal potential energy of the CNT is constant. Experimentation determined that CNTs in the XMD program reach mechanical equilibrium after seconds. 3 The output from the XMD program was strain energy, not strain energy density. This is why, after taking the second derivative, the resulting value was not Young s modulus, but was the product of Young s modulus and atomic volume. 6
7 Figure 3: Young s moduli for the three CNT chiralities of different lengths. The maximum strain that the CNTs experienced in the simulation that produced the data for this graph was.01, but very similar trends appeared in simulations of CNTs under all levels of strain. 7
8 (5,5) armchair CNT ± TPa (9,0) zigzag CNT ± TPa (6,4) chiral CNT ± TPa Table 1: Estimated values for Young s modulus of CNTs calculated with the definition of Y. (5,5) armchair CNT ± TPa (9,0) zigzag CNT ± TPa (6,4) chiral CNT ± TPa Table 2: Values for Young s modulus of CNTs under various strains calculated with the new method. In order to check the reliability of the simulations that produced these results, Young s modulus was also derived by using the definition of Young s modulus: Y = σ. Since the ε internal stress is a response to the strain, the applied axial stress σ could be estimated from it. Then, the strain ε was graphed against the stress σ, andtheslopeoftheresultingline, which is Young s modulus Y,wascalculated. OnlyresultinglinesthathadR were considered valid and below the yield point of the CNT, and so only CNTs experiencing strains of.04 or less were considered. The results of this check are listed in Table 1. The resulting Young s moduli from the simulations are listed in Table 2. They correlate closely with the data in Table 1, confirming the accuracy of the results. Experimental data sets the estimated Young s modulus of any given CNT is around 1 TPa [3]. So, the results in Table 2 are also in agreement with the experimental data. 5 Future Directions The XMD program created for this project can be used as a base for many other simulations involving CNTs. For example, future work could examine the effects of temperature or chirality on Young s modulus. Since the program created during this project and the results it produced are reliable, the relationship between applied axial stress and the resulting axial strain can be calculated for CNTs of any chirality. This ability to correlate stress and strain removes one of the major obstacles preventing the use of CNTs in many practical applications. Now that more is known about the mechanical properties of CNTs, future work could begin to relate the mechanical properties with other properties of CNTs, such as electrical properties of the nanotubes. 8
9 References [1] M. Monthioux & V. L. Kuznetsov, Carbon 44, 9(2006). [2] B. P. Grady. < [3] J. P. Lu, Phys. Rev. Lett. 79, 7(1997). [4] M.F. Yu et al., Science 287, 5453(2000). [5] C. P. Poole & F. J. Owens, Introduction to Nanotechnology, Wiley (2003). [6] X. Wang et al., Nano Lett. 9, 9(2009). [7] X. Lu & Z. Chen, Chem. Rev., 105, 10(2005). [8] S. Price, Science News (2000). Audacious & Outrageous: Space Elevators. < 1/> [9] A. E. Aliev et al., Science 323, 5921(2009). [10] R. Sanders, UC Berkeley News (2003). Physicists build world s smallest motor using nanotubes and etched silicon. < motor.shtml> [11] S. Heinze et al., Phys. Rev. Lett. 89, 10(2002). [12] M. S. Dresselhaus & H. Dai, MRS Bulletin (2004). Carbon Nanotubes: Continued Innovations and Challenges. < [13] H. D. Young & R. Geller, College Physics (2006). < [14] V. N. Popov & V. E. Van Doren, Phys. Rev. B 61, 4(2000). [15] D. Vodnik. < 9
Quantized Electrical Conductance of Carbon nanotubes(cnts)
Quantized Electrical Conductance of Carbon nanotubes(cnts) By Boxiao Chen PH 464: Applied Optics Instructor: Andres L arosa Abstract One of the main factors that impacts the efficiency of solar cells is
More informationAli Nasir Imtani and V. K. Jindal Department of Physics, Panjab University, Changdigrah , India. Abstract
Bond Lengths of SingleWalled Carbon Nanotubes Ali Nasir Imtani and V. K. Jindal Department of Physics, Panjab University, Changdigrah6004, India. Abstract Results of the bond lengths for various chiralities
More informationCarbon Nanotubes (CNTs)
Carbon Nanotubes (s) Seminar: Quantendynamik in mesoskopischen Systemen Florian Figge Fakultät für Physik AlbertLudwigsUniversität Freiburg July 7th, 2010 F. Figge (University of Freiburg) Carbon Nanotubes
More informationWhy are we so excited about carbon nanostructures? Mildred Dresselhaus Massachusetts Institute of Technology Cambridge, MA
Why are we so excited about carbon nanostructures? Mildred Dresselhaus Massachusetts Institute of Technology Cambridge, MA Conference for Undergraduate Women in Physics at Yale January 18, 2009 Why are
More informationIntensity (a.u.) Intensity (a.u.) Raman Shift (cm 1 ) Oxygen plasma. 6 cm. 9 cm. 1mm. Singlelayer graphene sheet. 10mm. 14 cm
Intensity (a.u.) Intensity (a.u.) a Oxygen plasma b 6 cm 1mm 10mm Singlelayer graphene sheet 14 cm 9 cm Flipped Si/SiO 2 Patterned chip Plasmacleaned glass slides c d After 1 sec normal Oxygen plasma
More informationFUTURISTIC MATERIALS BASED ON CARBON NANOTUBES FOR DEFENCE APPICATIONS A CASE STUDY
FUTURISTIC MATERIALS BASED ON CARBON NANOTUBES FOR DEFENCE APPICATIONS A CASE STUDY Abrar Shaik 1 and Revanasiddappa 2* 1 Department of Mechanical Engineering, 2 Department of Engineering Chemistry, Hosur
More informationNonlocal material properties of single walled carbon nanotubes
Nonlocal material properties of single walled carbon nanotubes J. V. Araújo dos Santos * and C. M. Mota Soares IDMEC, Instituto Superior Técnico, Universidade Técnica de Lisboa, Portugal Av. Rovisco Pais,
More informationChapter 1: Introduction of Carbon Nanotubes: Properties, Synthesis, Characterization and Applications
Chapter 1: Introduction of Carbon Nanotubes: Properties, Synthesis, Characterization and Applications 1.1. Background 1.2. Introduction of carbon and their allotropes 1.3. Carbon nanotubes (CNTs) 1.4.
More informationChapter 3. The structure of crystalline solids 3.1. Crystal structures
Chapter 3. The structure of crystalline solids 3.1. Crystal structures 3.1.1. Fundamental concepts 3.1.2. Unit cells 3.1.3. Metallic crystal structures 3.1.4. Ceramic crystal structures 3.1.5. Silicate
More informationTEMPERATURE DEPENDENCE OF THE TENSILE PROPERTIES OF SINGLE WALLED CARBON NANOTUBES: O(N) TIGHT BINDING MD SIMULATION GÜLAY DERELİ *, BANU SÜNGÜ
TEMPERATURE DEPENDENCE OF THE TENSILE PROPERTIES OF SINGLE WALLED CARBON NANOTUBES: O(N) TIGHT BINDING MD SIMULATION GÜLAY DERELİ *, BANU SÜNGÜ Department of Physics, Yildiz Technical University, 34210
More informationHydrogen Storage in Single and Multiwalled Carbon Nanotubes and Nanotube Bundles
Australian Journal of Basic and Applied Sciences, 5(7): 483490, 2011 ISSN 19918178 Hydrogen Storage in Single and Multiwalled Carbon Nanotubes and Nanotube Bundles 1 S. Hamidi and 2 H. Golnabi 1 Physics
More informationGraphene and Carbon Nanotubes
Graphene and Carbon Nanotubes 1 atom thick films of graphite atomic chicken wire Novoselov et al  Science 306, 666 (004) 100μm Geim s group at Manchester Novoselov et al  Nature 438, 197 (005) KimStormer
More informationThe many forms of carbon
The many forms of carbon Carbon is not only the basis of life, it also provides an enormous variety of structures for nanotechnology. This versatility is connected to the ability of carbon to form two
More informationMOLECULAR DYNAMICS SIMULATION OF HYDROGEN STORAGE IN SINGLEWALLED CARBON NANOTUBES
MOLECULAR DYNAMICS SIMULATION OF HYDROGEN STORAGE IN SINGLEWALLED CARBON NANOTUBES Shigeo MARUYAMA Engineering Research Institute The University of Tokyo 21116 Yayoi, Bunkyoku, Tokyo 1138656, Japan
More informationUnderstanding Irreducible and Reducible Oxides as Catalysts for Carbon Nanotubes and Graphene Formation
Wright State University CORE Scholar Special Session 5: Carbon and Oxide Based Nanostructured Materials (2011) Special Session 5 62011 Understanding Irreducible and Reducible Oxides as Catalysts for Carbon
More informationphysical Carbon Nanotubes Properties of Physical Properties of Carbon Nanotubes Downloaded from
physical Properties of Carbon Nanotubes This page is intentionally left blank Rysical Properties of Carbon Nanotubes GDRESSELElAUS & M S DRBSELMUS MZT Imperial College Press Published by Imperial College
More informationLectures Graphene and
Lectures 1516 Graphene and carbon nanotubes Graphene is atomically thin crystal of carbon which is stronger than steel but flexible, is transparent for light, and conducts electricity (gapless semiconductor).
More informationIntroduction to Nanotechnology Chapter 5 Carbon Nanostructures Lecture 1
Introduction to Nanotechnology Chapter 5 Carbon Nanostructures Lecture 1 ChiiDong Chen Institute of Physics, Academia Sinica chiidong@phys.sinica.edu.tw 02 27896766 Carbon contains 6 electrons: (1s) 2,
More informationSynthesis of nanotubes. Ewelina Broda
Synthesis of nanotubes Ewelina Broda Presentation Overview 1. Introduction 2. History 3. Types and structures 4. Properties 5. Synthesis 6. Applications 7. References Allotropes of Elemental Carbon History
More informationComputer Simulations of Carbon Nanostructures under Pressure
Fullerenes, Nanotubes, and Carbon Nanostructures, 13: 13 20, 2005 Copyright # Taylor & Francis, Inc. ISSN 1536383X print/15364046 online DOI: 10.1081/FST200039164 Computer Simulations of Carbon Nanostructures
More informationElasticity: Term Paper. Danielle Harper. University of Central Florida
Elasticity: Term Paper Danielle Harper University of Central Florida I. Abstract This research was conducted in order to experimentally test certain components of the theory of elasticity. The theory was
More informationNonlinear Mechanics of Monolayer Graphene Rui Huang
Nonlinear Mechanics of Monolayer Graphene Rui Huang Center for Mechanics of Solids, Structures and Materials Department of Aerospace Engineering and Engineering Mechanics The University of Texas at Austin
More informationRefering to Fig. 1 the lattice vectors can be written as: ~a 2 = a 0. We start with the following Ansatz for the wavefunction:
1 INTRODUCTION 1 Bandstructure of Graphene and Carbon Nanotubes: An Exercise in Condensed Matter Physics developed by Christian Schönenberger, April 1 Introduction This is an example for the application
More informationIV characteristics model for Carbon Nanotube Field Effect Transistors
International Journal of Engineering & Technology IJETIJENS Vol:14 No:04 33 IV characteristics model for Carbon Nanotube Field Effect Transistors Rebiha Marki, Chérifa Azizi and Mourad Zaabat. Abstract
More informationA General Equation for Fitting Contact Area and Friction vs Load Measurements
Journal of Colloid and Interface Science 211, 395 400 (1999) Article ID jcis.1998.6027, available online at http://www.idealibrary.com on A General Equation for Fitting Contact Area and Friction vs Load
More informationImaging Carbon materials with correlative RamanSEM microscopy. Introduction. Raman, SEM and FIB within one chamber. Diamond.
Imaging Carbon materials with correlative RamanSEM microscopy Application Example Carbon materials are widely used in many industries for their exceptional properties. Electric conductance, light weight,
More informationManipulating Graphene at the Atomicscale
Manipulating Graphene at the Atomicscale Mike Crommie Dept. of Physics, UC Berkeley Materials Science Division, LBNL (I) Atomicscale Gating  Tunable charge centers (II) Nanoribbon Edge States  Controllable
More informationPIC/MCC Simulation of Radio Frequency Hollow Cathode Discharge in Nitrogen
PIC/MCC Simulation of Radio Frequency Hollow Cathode Discharge in Nitrogen HAN Qing ( ), WANG Jing ( ), ZHANG Lianzhu ( ) College of Physics Science and Information Engineering, Hebei Normal University,
More informationstatus solidi Department of Physics, University of California at Berkeley, Berkeley, CA, USA 2
physica pss status solidi basic solid state physics b Extreme thermal stability of carbon nanotubes G. E. Begtrup,, K. G. Ray, 3, B. M. Kessler, T. D. Yuzvinsky,, 3, H. Garcia,,, 3 and A. Zettl Department
More informationNanofabrication/NanoCharacterization Calixarene and CNT Control Technology
Nanofabrication/NanoCharacterization Calixarene and CNT Control Technology ISHIDA Masahiko, FUJITA Junichi, NARIHIRO Mitsuru, ICHIHASHI Toshinari, NIHEY Fumiyuki, OCHIAI Yukinori Abstract The world of
More informationCMOS Scaling. Two motivations to scale down. Faster transistors, both digital and analog. To pack more functionality per area. Lower the cost!
Two motivations to scale down CMOS Scaling Faster transistors, both digital and analog To pack more functionality per area. Lower the cost! (which makes (some) physical sense) Scale all dimensions and
More information18 Carbon Nanotubes Introduction. Meyya Meyyappan. Deepak Srivastava
18 Carbon Nanotubes Meyya Meyyappan NASA Ames Research Center Deepak Srivastava NASA Ames Research Center CONTENTS 18.1 Introduction 18.2 Structure and Properties of Carbon Nanotubes 18.3 Computational
More informationOrigins, Properties, and Applications of Carbon Nanotubes and Fullerenes
Origins, Properties, and Applications of Carbon Nanotubes and Fullerenes by Mario Anthony Rosso Submitted in partial fulfillment of the requirements for the graduate course IT 283 Advance Materials and
More informationInternal lattice relaxation of singlelayer graphene under inplane deformation. Jun Zhou and Rui Huang
Internal lattice relaxation of singlelayer graphene under inplane deformation Jun Zhou and Rui Huang Department of Aerospace Engineering and Engineering Mechanics, University of Texas, Austin, TX 7871
More informationChapter 2 Carbon Nanotubes
Chapter 2 Carbon Nanotubes 2.1 Introduction Carbon nanotubes have attracted significant attention since their discovery, as unique valuable nanostructures, with many outstanding properties, leading them
More informationNovel Dispersion and SelfAssembly
Novel Dispersion and SelfAssembly of Carbon Nanotubes Mohammad F. Islam 100g Department of Chemical Engineering and Department of Materials Science & Engineering Funding Agencies http://islamgroup.cheme.cmu.edu
More informationNanotechnology. Yung Liou P601 Institute of Physics Academia Sinica
Nanotechnology Yung Liou P601 yung@phys.sinica.edu.tw Institute of Physics Academia Sinica 1 1st week Definition of Nanotechnology The Interagency Subcommittee on Nanoscale Science, Engineering and Technology
More informationConductivity in Carbon Nanotubes Stephen French
Conductivity in Carbon Nanotubes Stephen French Abstract Vapor deposition is explored as a means of directly lowering the resistance of thin films of carbon nanotubes. In the process, atmospheric doping
More informationTransversal electric field effect in multilayer graphene nanoribbon
Transversal electric field effect in multilayer graphene nanoribbon S. Bala kumar and Jing Guo a) Department of Electrical and Computer Engineering, University of Florida, Gainesville, Florida 32608, USA
More informationDiamond. There are four types of solid: Hard Structure  Tetrahedral atomic arrangement. What hybrid state do you think the carbon has?
Bonding in Solids Bonding in Solids There are four types of solid: 1. Molecular (formed from molecules)  usually soft with low melting points and poor conductivity. 2. Covalent network  very hard with
More information1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine Spring 2004 LABORATORY ASSIGNMENT NUMBER 6
1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine MIT Spring 2004 LABORATORY ASSIGNMENT NUMBER 6 COMPRESSION TESTING AND ANISOTROPY OF WOOD Purpose: Reading: During this laboratory
More informationCarbon Nanomaterials: Nanotubes and Nanobuds and Graphene towards new products 2030
Carbon Nanomaterials: Nanotubes and Nanobuds and Graphene towards new products 2030 Prof. Dr. Esko I. Kauppinen Helsinki University of Technology (TKK) Espoo, Finland Forecast Seminar February 13, 2009
More information4.2.1 Chemical bonds, ionic, covalent and metallic
4.2 Bonding, structure, and the properties of matter Chemists use theories of structure and bonding to explain the physical and chemical properties of materials. Analysis of structures shows that atoms
More informationCarbon nanotubes synthesis. Ing. Eva Košťáková KNT, FT, TUL
Carbon nanotubes synthesis Ing. Eva Košťáková KNT, FT, TUL Basic parameters: Temperature (500, 1000 C ) Pressure (normal, vacuum ) Gas (ambient, inert atmosphere nitrogen, argon ) Time (duration, time
More informationGraphene edge from A to Z and the origins of nanotube chirality
Graphene edge from A to Z and the origins of nanotube chirality Yuanyue Liu, Alex Dobrinsky, and Boris I. Yakobson Department of Mechanical Engineering & Materials Science, Department of Chemistry, and
More informationMATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?
MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition
More informationStress analysis of a stepped bar
Stress analysis of a stepped bar Problem Find the stresses induced in the axially loaded stepped bar shown in Figure. The bar has crosssectional areas of A ) and A ) over the lengths l ) and l ), respectively.
More informationCVD growth of Graphene. SPE ACCE presentation Carter Kittrell James M. Tour group September 9 to 11, 2014
CVD growth of Graphene SPE ACCE presentation Carter Kittrell James M. Tour group September 9 to 11, 2014 Graphene zigzag armchair History 1500: PencilIs it made of lead? 1789: Graphite 1987: The first
More informationNanotechnology 5 th lecture
Nanotechnology 5 th lecture (c) http://www.nccrnano.org/nccr_data/ gallery/gallery_01/gallery_01_03/pics_06/ internet/nanotube_spiral.jpg Plan for today: http://www.nccrnano.org/nccr_data/gallery/ gallery_01/gallery_01_03/pics_04/internet/
More information1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor.
Elasticity Homework Problems 2014 Section 1. The Strain Tensor. 1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor. 2. Given a steel bar compressed with a deformation
More informationConference Return Seminar NANO2014,Moscow State University,Moscow,Russia Date: th July 2014
Conference Return Seminar NANO2014,Moscow State University,Moscow,Russia Date:131818 th July 2014 An electrochemical method for the synthesis of single and few layers graphene sheets for high temperature
More informationStudy on the Microwave Permeability of the CNT Complex in 218GHz
Study on the Microwave Permeability of the CNT Complex in 218GHz Qinghuai Li & Xiaolai Liu (Corresponding author) College of Science, University of Chemical Industry of Beijing, Beijing 100029, China
More informationDefense Technical Information Center Compilation Part Notice
UNCLASSIFIED Defense Technical Information Center Compilation Part Notice ADP012151 TITLE: Chemical Bonding of Polymer on Carbon Nanotube DISTRIBUTION: Approved for public release, distribution unlimited
More information1/2. E c Part a The solution is identical for grade 40 and grade 60 reinforcement. P s f c n A s lbf. The steel carries 13.3 percent of the load
1/2 3.1. A 16 20 in. column is made of the same concrete and reinforced with the same six No. 9 (No. 29) bars as the column in Examples 3.1 and 3.2, except t hat a steel with yield strength f y = 40 ksi
More informationARCHITECTURE AND CAD FOR CARBON NANOMATERIAL INTEGRATED CIRCUITS SCOTT ERICK CHILSTEDT THESIS
ARCHITECTURE AND CAD FOR CARBON NANOMATERIAL INTEGRATED CIRCUITS BY SCOTT ERICK CHILSTEDT THESIS Submitted in partial fulfillment of the requirements for the degree of Master of Science in Electrical and
More informationChapter 12. Static Equilibrium and Elasticity
Chapter 12 Static Equilibrium and Elasticity Static Equilibrium Equilibrium implies that the object moves with both constant velocity and constant angular velocity relative to an observer in an inertial
More informationArcsynthesis of Singlewalled Carbon Nanotubes in Nitrogen Atmosphere
Fullerenes, Nanotubes and Carbon Nanostructures, 16: 330 334, 2008 Copyright # Taylor & Francis Group, LLC ISSN 1536383X print/15364046 online DOI: 10.1080/15363830802219849 Arcsynthesis of Singlewalled
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationMechanics of Irregular Honeycomb Structures
Mechanics of Irregular Honeycomb Structures S. Adhikari 1, T. Mukhopadhyay 1 Chair of Aerospace Engineering, College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP, UK Sixth International
More informationProperties of carbon nanotubes under external factors: Adsorption, mechanical deformations, defects, and external electric fields
University of South Florida Scholar Commons Graduate Theses and Dissertations Graduate School 21 Properties of carbon nanotubes under external factors: Adsorption, mechanical deformations, defects, and
More informationSUPPLEMENTARY INFORMATION
Ultrahigh interlayer friction in multiwalled boron nitride nanotubes 1 Contents Nanotubes production and characterizations 2 Experimental Methods 4 Post mortem characterization of the nanotubes 4 Références
More informationAn Extended Hückel Theory based Atomistic Model for Graphene Nanoelectronics
Journal of Computational Electronics X: YYYZZZ,? 6 Springer Science Business Media, Inc. Manufactured in The Netherlands An Extended Hückel Theory based Atomistic Model for Graphene Nanoelectronics HASSAN
More informationThermal Expansion of Single Wall Carbon Nanotubes
H. Jiang B. Liu Y. Huang Department of Mechanical and Industrial Engineering, University of Illinois, Urbana, IL 61801 K. C. Hwang Department of Engineering Mechanics, Tsinghua University, Beijing, China
More informationSCIENCE & TECHNOLOGY
Pertanika J. Sci. & Technol. 25 (S): 205212 (2017) SCIENCE & TECHNOLOGY Journal homepage: http://www.pertanika.upm.edu.my/ Effect of Boron and Oxygen Doping to Graphene Band Structure Siti Fazlina bt
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationNOVEL STRUCTURES FOR CARBON NANOTUBE FIELD EFFECT TRANSISTORS
International Journal of Modern Physics B Vol. 23, No. 19 (2009) 3871 3880 c World Scientific Publishing Company NOVEL STRUCTURES FOR CARBON NANOTUBE FIELD EFFECT TRANSISTORS RAHIM FAEZ Electrical Engineering
More informationFLUID FLOW THROUGH CARBON NANOTUBES: A NEW MODELING AND SIMULATION APPROACH. A Thesis. Presented to. The Graduate Faculty of The University of Akron
FLUID FLOW THROUGH CARBON NANOTUBES: A NEW MODELING AND SIMULATION APPROACH A Thesis Presented to The Graduate Faculty of The University of Akron In Partial Fulfillment of the Requirements for the Degree
More informationMolecular Dynamics Study of Thermal Rectification in Graphene Nanoribbons
Molecular Dynamics Study of Thermal Rectification in Graphene Nanoribbons Jiuning Hu 1* Xiulin Ruan 2 Yong P. Chen 3# 1School of Electrical and Computer Engineering and Birck Nanotechnology Center, Purdue
More informationChapter 12: Structures & Properties of Ceramics
Chapter 12: Structures & Properties of Ceramics ISSUES TO ADDRESS... How do the crystal structures of ceramic materials differ from those for metals? How do point defects in ceramics differ from those
More informationchiral m = n Armchair m = 0 or n = 0 Zigzag m n Chiral Three major categories of nanotube structures can be identified based on the values of m and n
zigzag armchair Three major categories of nanotube structures can be identified based on the values of m and n m = n Armchair m = 0 or n = 0 Zigzag m n Chiral Nature 391, 59, (1998) chiral J. Tersoff,
More informationDependence of the electrical properties of defective singlewalled carbon nanotubes on the vacancy density
Dependence of the electrical properties of defective singlewalled carbon nanotubes on the vacancy density Luo YuPin( ) a), Tien LiGan( ) b), Tsai ChuenHorng( ) b), Lee MingHsien( ) c), and Li FengYin(
More informationFREE VIBRATION ANALYSIS OF THIN CYLINDRICAL SHELLS SUBJECTED TO INTERNAL PRESSURE AND FINITE ELEMENT ANALYSIS
FREE VIBRATION ANALYSIS OF THIN CYLINDRICAL SHELLS SUBJECTED TO INTERNAL PRESSURE AND FINITE ELEMENT ANALYSIS J. Kandasamy 1, M. Madhavi 2, N. Haritha 3 1 Corresponding author Department of Mechanical
More informationNanostrukturphysik Übung 2 (Class 3&4)
Nanostrukturphysik Übung 2 (Class 3&4) Prof. Yong Lei & Dr. Yang Xu 2017.05.03 Fachgebiet 3DNanostrukturierung, Institut für Physik Contact: yong.lei@tuilmenau.de (3748), yang.xu@tuilmenau.de (4902)
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationPHY 481/581. Some classical/quantum physics for the nanometer length scale.
PHY 481/581 Some classical/quantum physics for the nanometer length scale http://creativecommons.org/licenses/byncsa/3.0/ 1 What is nanoscience? the science of materials whose properties scale with
More informationClar Sextet Theory for lowdimensional carbon nanostructures: an efficient approach based on chemical criteria
Clar Sextet Theory for lowdimensional carbon nanostructures: an efficient approach based on chemical criteria Matteo Baldoni Fachbereich Chemie, Technische Universität Dresden, Germany Department of Chemistry
More informationEquilibrium & Elasticity
PHYS 101 Previous Exam Problems CHAPTER 12 Equilibrium & Elasticity Static equilibrium Elasticity 1. A uniform steel bar of length 3.0 m and weight 20 N rests on two supports (A and B) at its ends. A block
More informationNANO TECHNOLOGY IN POLYMER SOLAR CELLS. Mayur Padharia, Hardik Panchal, Keval Shah, *Neha Patni, Shibu.G.Pillai
NANO TECHNOLOGY IN POLYMER SOLAR CELLS Mayur Padharia, Hardik Panchal, Keval Shah, *Neha Patni, Shibu.G.Pillai Department of Chemical Engineering, Institute of Technology, Nirma University, S. G. Highway,
More informationChapter II: Reversible process and work
Chapter II: Reversible process and work 1 Process Defined by change in a system, a thermodynamic process is a passage of a thermodynamic system from an initial to a final state of thermodynamic equilibrium.
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationInteraction between Singlewalled Carbon Nanotubes and Water Molecules
Workshop on Molecular Thermal Engineering Univ. of Tokyo 2013. 07. 05 Interaction between Singlewalled Carbon Nanotubes and Water Molecules Shohei Chiashi Dept. of Mech. Eng., The Univ. of Tokyo, Japan
More information7. Carbon Nanotubes. 1. Overview: Global status market price 2. Types. 3. Properties. 4. Synthesis. MWNT / SWNT zigzag / armchair / chiral
7. Carbon Nanotubes 1. Overview: Global status market price 2. Types MWNT / SWNT zigzag / armchair / chiral 3. Properties electrical others 4. Synthesis arc discharge / laser ablation / CVD 5. Applications
More informationGraphene Novel Material for Nanoelectronics
Graphene Novel Material for Nanoelectronics Shintaro Sato Naoki Harada Daiyu Kondo Mari Ohfuchi (Manuscript received May 12, 2009) Graphene is a flat monolayer of carbon atoms with a twodimensional honeycomb
More informationSolid State. Subtopics
01 Solid State Chapter 01: Solid State Subtopics 1.0 Introduction 1.1 Classification of solids 1.2 Classification of crystalline solids 1.3 Unit cell, two and three dimensional lattices and number of atoms
More informationJeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA UNESCO EOLSS
MECHANICS OF MATERIALS Jeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA Keywords: Solid mechanics, stress, strain, yield strength Contents 1. Introduction 2. Stress
More informationAb initio study of CNT NO 2 gas sensor
Chemical Physics Letters 387 (2004) 271 276 www.elsevier.com/locate/cplett Ab initio study of CNT NO 2 gas sensor Shu Peng a, *, Kyeongjae Cho a, Pengfei Qi b, Hongjie Dai b a Department of Mechanical
More informationFlitched Beams. Strain Compatibility. Architecture 544 Wood Structures. Strain Compatibility Transformed Sections Flitched Beams
Architecture 544 Wood Structures Flitched Beams Strain Compatibility Transformed Sections Flitched Beams University of Michigan, TCAUP Structures II Slide 1/27 Strain Compatibility With two materials bonded
More informationLOWER FREQUENCY LIMIT OF CARBON NANOTUBE ANTENNA
Progress In Electromagnetics Research, PIER 94, 419 433, 2009 LOWER FREQUENCY LIMIT OF CARBON NANOTUBE ANTENNA A. M. Attiya Electronics Research Institute, Microwave Engineering Department ElTahreer St.,
More informationImpact of size and temperature on thermal expansion of nanomaterials
PRAMANA c Indian Academy of Sciences Vol. 84, No. 4 journal of April 205 physics pp. 609 69 Impact of size and temperature on thermal expansion of nanomaterials MADAN SINGH, and MAHIPAL SINGH 2 Department
More informationUNIVERSITY PHYSICS I. Professor Meade Brooks, Collin College. Chapter 12: STATIC EQUILIBRIUM AND ELASTICITY
UNIVERSITY PHYSICS I Professor Meade Brooks, Collin College Chapter 12: STATIC EQUILIBRIUM AND ELASTICITY Two stilt walkers in standing position. All forces acting on each stilt walker balance out; neither
More informationAnalysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements
Acta Mech. Sin. (2016) 32(2):295 300 DOI 10.1007/s1040901505342 RESEARCH PAPER Analysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements V. H. Carneiro 1
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationDoctoral School in Materials Engineering XXII cycle
Doctoral School in Materials Engineering XXII cycle Surface Engineering for Microsensing Luca Minati January 2010 Surface Engineering for Microsensing Author Minati Luca Tutors Prof. Claudio Migliaresi
More informationInvestigation on the growth of CNTs from SiO x and Fe 2 O 3 nanoparticles by in situ TEM
The 5 th Workshop on Nucleation and Growth Mechanisms of SWCNTs Investigation on the growth of CNTs from SiO x and Fe 2 O 3 nanoparticles by in situ TEM Chang Liu Shenyang National Laboratory for Materials
More informationEnhancement of the Properties of Polymer by using Carbon Nanotubes
University of New Orleans ScholarWorks@UNO University of New Orleans Theses and Dissertations Dissertations and Theses 12202009 Enhancement of the Properties of Polymer by using Carbon Nanotubes WaiYin
More informationCHARACTERIZING MECHANICAL PROPERTIES OF GRAPHITE USING MOLECULAR DYNAMICS SIMULATION
CHARACTERIZING MECHANICAL PROPERTIES OF GRAPHITE USING MOLECULAR DYNAMICS SIMULATION JiaLin Tsai and JieFeng Tu Department of Mechanical Engineering, National Chiao Tung University 1001 University Road,
More informationComputer simulation of the Poisson's ratio of soft polydisperse discs at zero temperature
Computer simulation of the Poisson's ratio of soft polydisperse discs at zero temperature JAKUB NAROJCZYK KRZYSZTOF W. WOJCIECHOWSKI Institute of Molecular Physics Polish Academy of Sciences ul. M. Smoluchowskiego
More informationNumerical Modeling of Delamination Resistance Improvement Through The Use of CNTReinforced Bonding Layers
21 st International Conference on Composite Materials Xi an, 2025 th August 2017 Numerical Modeling of Delamination Resistance Improvement Through The Use of CNTReinforced Bonding Layers Yassine ElAssami
More informationEffect of strain on the band gap and effective mass of zigzag singlewall carbon nanotubes: Firstprinciples densityfunctional calculations
PHYSICAL REVIEW B 77, 1553 8 Effect of strain on the band gap and effective mass of zigzag singlewall carbon nanotubes: Firstprinciples densityfunctional calculations S. Sreekala, 1, * X.H. Peng, 1
More informationFor more information, please contact: or +1 (302)
Introduction Graphene Raman Analyzer: Carbon Nanomaterials Characterization Dawn Yang and Kristen Frano B&W Tek Carbon nanomaterials constitute a variety of carbon allotropes including graphene, graphene
More information